Chapter 7. Chips, Sawdust, Planer Shavings, Bark, and Hog Fuel


 Amy George
 2 years ago
 Views:
Transcription
1 Chapter 7. Chips, Sawdust, Planer Shavings, Bark, and Hog Fuel Expansion Factors, Relative Solid Volume, and Compaction 84 Expansion (Fluffing) Factor 84 Loose expansion factor Compacted expansion factor Relative Solid Volume 84 Compaction 84 Compaction ratio Compaction percent Summary 85 Bulk Density 85 Ovendry Bulk Density 85 Wet Bulk Density 85 Effect of Drying (Shrinkage) on Bulk Density 87 Summary 87 Units of Residue Measure and Conversions 87 The 200 Cubic Foot Volumetric Unit 87 Weight Measures 90 Stowage Factor and Compaction in Shipping 91 Stowage factor Compaction percent Residue Yield 91 Sawdust91 Pulp Chips 91 Planer Shavings 91 Bark 91 Hog Fuel 93 Residue Calculation Examples 93 Estimating Yield from Plywood 93 Estimating Yield per Cunit of Log Input 93 Converting Units of Residue to Weight 93 Estimating a Hog Fuel Mix 94 83
2
3 Chapter 7. Chips, Sawdust, Planer Shavings, Bark, and Hog Fuel Previous chapters have presented material balances that can be used to estimate the fraction of a log recovered in a residue form. There are many factors that affect chip and residue measures and associated conversion factors. These include: Size and geometry: The differences in physical characteristics of these residues are obvious and affect how they occupy a unit of space. Specific gravity: Wood and bark densities differ between species (Tables 11, 75). Moisture content: Wood and bark moisture contents vary between species (Table 11), and water may be added during pond storage and debarking. Buyers and sellers of residues and statistical reporting organizations generally devise some method for correcting to the ovendry state. Degree of compaction: Over time, chips and residues will settle due to gravity. Also, mechanical and pneumatic compaction can be used to pack more residue into a given space. Quantities of chips and residues are measured in units of volume or weight. This chapter discusses volumetric expansion factors and bulk densities for these products, typical units of measure and conversion, and residue yields, and also presents examples that integrate this material. Expansion Factors, Relative Solid Volume, and Compaction To illustrate these terms, consider a log containing 5 cubic feet of solid wood (Vsw) that is chipped. Obviously, the chips will occupy more space than 5 cubic feet. Expansion (Fluffing) Factor Loose Expansion Factor. Immediately after chipping, suppose the loose chips occupy 15 cubic feet (Vp). The expansion factor (E), also called the fluffing factor, is E (loose) = Vp / Vsw = 15 ft 3 / 5 ft 3 = Note that when Vsw and Vp are measured in cubic meters, the expansion factor has the same value. Compacted Expansion Factor. Loose chips will settle over time due to gravity, or they may be physically compacted by equipment. Suppose the chips are compacted so the space occupied (Vp) reduces to 12 cubic feet. The expansion factor is E (compacted) = 12 ft 3 / 5 ft 3 = These calculations illustrate the importance of noting the degree of compaction associated with a particular expansion factor. Measures of compaction are discussed below. Relative Solid Volume The reciprocal of the expansion factor measures the number of solid cubic feet (cubic meters) that will yield a cubic foot (cubic meter) of residue. Continuing the example, relative solid volume (RSV), also termed volume occupancy, is RSV (loose) = 1 / E (loose) = 1 / = RSV (compacted) = 1 / E (compacted) = 1 / 2.40 = Some multiply RSV by 100 to express it as a percentage; in this form it is sometimes called a compaction rate. Compaction Compaction Ratio. A common measure of compaction is the compaction ratio (CR), which is CR = Vp (loose) / Vp (compacted) = 15 ft 3 / 12 ft 3 = CR = E (loose) / E (compacted) = 3.00 / 2.40 = CR can also be calculated from the relative solid volumes. It has a value of one for loose residue and increases as the particles become more compacted. A maximum value for CR can be estimated if it is assumed that the maximum compaction possible would compress the residue to the original volume of solid wood. Under these conditions: Vp (compacted) = Vsw hence CR = 15 ft 3 / 5 ft 3 = Chips 3
4 In other words, the limiting value of the compaction ratio is numerically equal to the expansion factor for loose particles. Compaction Percent. A less common compaction value can be obtained from volume changes. From the example, the maximum compaction from loose chips to solid wood is 10 cubic feet, while the actual compaction is 3 cubic feet. Actual compaction as a percentage of the maximum possible is Compaction % = 100 * [Vp (loose) Vp (compacted)] / [Vp (loose) Vsw] = 100 * (15 12) / (15 5) = 30%. Summary Table 71 presents expansion factors for various types of residues and corresponding relative solid volumes. Also shown are conversions from Imperial to metric and equivalents when residues are measured in 200 cubic feet volumetric units (see p. 87). Tables 72 and 73 present additional sources of expansion factor and compaction ratios. The conversion methods applied to the expansion factors in Table 71 can also be applied to the expansion factors presented in Table 72. Bulk Density Bulk density (BD) refers to residue weight divided by residue volume. Suppose the example log has a moisture content of 80% MCod (44.4% MCw) and specific gravity (SGg) is 0.48 (see Chapter 1 for definitions). Using methods presented in Chapter 1, wood density is 53.9 wet pounds per green cubic foot. This is composed of 29.9 lb of ovendry wood plus 24.0 lb of water. The term basic density is sometimes used to refer to the ovendry weight per cubic foot (i.e., 29.9 lb/ft 3 ). The chips from the 5 cubicfoot log have the following weight distribution: Condition Weight (lb) Percent Ovendry wood (Wod) Water (MCw) Wood + water (Wwet) The term solids fraction refers to the percentage of total weight that is ovendry wood. As was described for solid wood density in Chapter 1, bulk density can be calculated for any combination of numerator (weight) and denominator (volume) moisture contents, hence it is important to specify these conditions. The more common cases are given in the remainder of this section. Ovendry Bulk Density This is the ovendry weight per green cubic foot of residue. Divide the weight of ovendry wood (Wod) by the residue volume (Vp) BDod (loose) = Wod / Vp (loose) = lb / 15 ft 3 = BDod (compacted) = Wod / Vp (compacted) = lb / 12 ft 3 = The same results can also be obtained by dividing the basic density (29.9 lb/ft 3 ) by the appropriate expansion factor. These bulk densities indicate the amount of ovendry wood present in each loose or compacted green cubic foot of residue. They are important in residue transactions because purchasers wish to pay only for wood and therefore want the weight of water excluded. The residue volume is green, since these are undried chips fresh from the log. In cases where residues are dried or manufactured from dry wood, these bulk densities would change because wood shrinkage will modify the volume the residue occupies. This will be illustrated below. Wet Bulk Density Bulk density can also be calculated with the moisture content included in the weight (total weight per green cubic foot of residue): BDwet (loose) = Wwet / Vp (loose) = (269.5 lb / 15 ft 3 ) = BDwet (compacted) = Wwet / Vp (compacted) = (269.5 lb / 12 ft 3 ) = The same results can also be obtained by dividing the wet wood density (53.9 lb/ft 3 ) by the appropriate expansion factor. These values are 4 Chapter 7
5 Chips 5
6 useful for estimating actual weights and loadings on equipment. For the same compaction, knowledge of moisture content allows conversion between BDod and BDwet: BDwet = BDod * (1 + MC od / 100). Effect of Drying (Shrinkage) on Bulk Density Bulk densities of dry residues or residues manufactured from dry wood will differ from those in the preceding example. One reason is that the type of residue may be different. Examples are planer shavings and sander dust obtained when kilndried wood is surfaced; these residue forms may have different expansion factors. Another reason is that because wood shrinks as it dries, the residue occupies less space. Since many secondary wood products industries, such as millwork and furniture, utilize dry wood, their ovendry bulk densities will be higher and their wet bulk densities will be lower due to the effects of shrinkage and lower moisture content. See Example 1. Summary This section has demonstrated how various factors affect bulk density calculations. Tables 72 and 73 present data illustrating the influence of mill source (residue type) and species on bulk densities. It should be obvious from the discussion that bulk density is ambiguous without clear statement of the species (wood specific gravity), type of residue, degree of compaction, and the moisture content of both the numerator and denominator. Units of Residue Measure and Conversions The 200 Cubic Foot Volumetric Unit A unit representing 200 cubic feet of space is a very common measure for residues. It is sometimes referred to as a gravity packed unit (GPU). Care should be taken when the word unit is used, since it may refer to other measures (e.g., bonedry unit in the next section). Example 1 Suppose 5 cubic feet of solid green wood is dried to 10% MCod (9.1% MC w ) and that the species has SGg = 0.48 and 15% total volumetric shrinkage. As seen in Chapter 1, shrinkage reduces the volume of solid wood to 4.5 cubic feet. If this dry wood is chipped with the same equipment that converted the green log into 15 cubic feet of green chips, the expansion factor of 3.00 predicts that the loose dry chips will occupy 13.5 cubic feet. The same result is obtained by applying volumetric shrinkage to the drying of the green chips to 10% MC od. If the dry chips are compacted to the same degree as the green chips, the compacted volume is 10.8 cubic feet. Using the methods explained in Chapter 1, we will find the weight density of this dry wood to be lb/ft 3. Of this, 33.2 pounds are ovendry wood and 3.35 pounds are water. The weight distribution of the dry chips is Condition Weight (lb) Percent Ovendry wood (W od) Water (MC w) Wood + water (W wet) Note that the solids fraction has risen to 90.9%. Using the previously calculated expansion factor for loose chips, bulk densities are BD od (loose) = lb / 13.5 ft 3 = BD wet (loose) = lb / 13.5 ft 3 = Calculations for compacted chips are similar except the compacted chip volume of 10.8 cubic feet is substituted. These results can also be obtained by dividing "basic" and wet wood densities by the loose expansion factor. Note that the cubic foot volume here refers to volume that remains after shrinkage to 10% MC od rather than the original green volume. The difference between the ovendry and wet bulk densities has narrowed. The ovendry bulk density increased because the volume occupied by the dry wood is less. The wet bulk density is also based on the smaller volume occupancy, but this is offset by the great reduction in weight of water. Hence the net effect is for the wet bulk density to decrease. The solid equivalent of a unit varies depending on particle geometry and degree of compaction. Table 71, column 7, divides the expansion factors into 200 to estimate the number of solid cubic feet of wood (or bark) that will expand to fill a unit. 6 Chapter 7
7 Chips 7
8 8 Chapter 7
9 Table 73. Average moisture content (MC w ) and bulk density of various wood residues. Bulk density (lb/ft 3 ) Green Ovendry Residue MC w Mean SE Mean SE U.S. South Hardwood sawdust and bark Mixed pinehardwood sawdust Clean hardwood pulp chips Hardwood wholetree chips Pine wholetree chips Hogged dry trims (hardwood) Shavings (hardwood) Western Ovendry density (lb/ft 3 ) Hogged fuel Sawdust Bark Secondary mill sawdust Shavings Sources: U.S. South: Harris and Phillips (1989). Western: Risbrut and Ellis (1981). SE = standard error. Column 9 presents reciprocals of column 7 (i.e., number of units that will result when one solid cubic foot is converted into the corresponding residue type). Column 8 presents the metric counterpart to column 7 (i.e., the number of solid cubic meters that will expand to fill a cubic meter of space with the particular residue). Conversions: 1 unit = 200 ft 3 = 5.66 m 3. 1 m 3 = ft 3 = unit. Weight Measures The common weight measures and conversions used in transactions and in various statistical sources are shown in Table 74. The weight of a bonedry unit (BDU) was obtained by experimentally weighing a number of cords of Douglasfir slab wood that were dried to 3 to 7% moisture content. The average weight, nearly 2,400 pounds, has become a standard basis for measuring residues. Of these weight measures, the long ton is the least common but is found in some statistical reports. Due to moisture content variation, weights are generally corrected to a zero percent moisture content (ovendry or bonedry). Consequently, actual shipping weight will be much greater. Two useful conversions are (Appendix 1, Table 2): To convert lb/ft 3 to kg/m 3 multiply by To convert kg/m 3 to lb/ft 3 multiply by Table 74. Residue weight measures and conversions. Short Long Ovendry (lb) Ovendry (kg) ton ton BDU Tonne Short ton 2, Long ton 2, BDU 2,400 1, Tonne 2, , Source: Calculated by the author. Chips 9
10 Stowage Factor and Compaction in Shipping Since wood chips and residues are light in weight, compaction is very important to minimize the transporation cost per ton. Stowage Factor. This is a marine term that measures the cubic volume of cargo space for products of known weights. It represents the number of cubic feet required, including void space, to contain a long ton of a product. Therefore, a stowage factor of 120 means that 120 cubic feet of space is needed to stow a long ton of a particular product. Compaction Percent. Because of variability in moisture content, stowage factors for chips are not reliable and an alternative, compaction percent, is more commonly used. Compaction means the packing of chips so the voids are minimized. The pulp and paper industry defines compaction as the number of bonedry units (BDU) that can be placed in a 200 cubic foot space. Thus one faces the potentially confusing situation relating BDU (a weight measure) to GPU (a volume measure). Compaction is usually expressed as a percentage. A 100% compaction means that a BDU occupies exactly 200 cubic feet, which implies a bulk density of 2,400 lb/200 ft 3 = 12 lb/ft 3. Similarly, 90% compaction means that 0.90 BDU occupies 200 cubic feet (bulk density = 10.8 lb/ft 3 ). With modern shiploading equipment, compaction percentages of 100% or more are commonly achieved. Compaction percent can be calculated by one of the following formulas. Compaction percent = 100 * BDU * 200 / ship volume, ft 3 = (long tons loaded) * 1.12 (100 MCw) * 200 / (1.2 * ship volume, ft3 ) = 2,240 * 200 * (100 MCw) / (stowage factor * 2,400) = (100 MCw) / stowage factor. Residue Yield The volume of sawdust produced in manufacturing lumber depends on sawkerf thickness, product line (number of saw cut lines), and log diameter. For a given log size and sawkerf, a mill producing smaller lumber items will generate more sawdust than a mill cutting large timbers. The material balance references in Chapter 4 are a good source of average sawdust yields in solid wood equivalent. The sawdust expansion factor in Table 71 or 72 should be applied to convert these solid wood equivalents to volume of sawdust as shipped. Pulp Chips Pulp chips are obtained from three principal sources: (1) whole logs, (2) sawmill slabs, edgings, and trimmings, and (3) veneer mill scraps and peeler cores, if the latter are not sold to stud sawmills or preservative plants for posts. The material balances in Chapters 4 and 5 provide estimates of average chip yields in solid wood equivalent from these processes. The chip expansion factor in Table 71 or 72 should be applied to convert these solid wood equivalents to volume of chips as shipped. The material balances assume that residues recovered as chips are fully utilized by pulp mills. Actually, a reject loss on the order of 2 to 5% will occur during pulp chip screening. This reject loss will be at the upper or lower end of this range depending on the condition of the chipper, the chip specification, and whether oversize chips are rechipped. Planer Shavings The volume of planer shavings obtained depends on the fraction of lumber output that is planed and the difference between the rough and surfaced dimensions. The material balances and computational methods in Chapter 4 can be used to estimate average shaving yields. Since these material balance estimates are in solid wood form, the expansion factor in Table 71 or 72 must be applied to get volume as shipped. Bark Bark volume varies with species, position on the tree, and tree size. Average bark volume can be Sawdust 10
11 Table 75. Bark contents of western species. Inner bark Outer bark Bark volume, % of % of percent of total total Species Wood Total bark MCod% SGg bark MCod% SGg SOFTWOODS Cedar Western redcedar Yellow (Alaska) Douglasfir Fir, true Hemlock, western Pine Lodgepole Ponderosa Western white Spruce Engelmann Sitka HARDWOODS Red alder Aspen Birch Black cottonwood Bigleaf maple Source: Smith and Kozak (1971). estimated either as a percent of total volume (including bark) or as a percent of wood volume: Bark volume as a percent of total volume (BTV%) = (dob 2 dib 2 ) / dob 2 * 100 Bark volume as a percent of wood volume (BWV%) = (dob 2 dib 2 ) / dib 2 * 100 where dob = diameter outside bark dib = diameter inside bark. For example, for a log measuring 20 inches in diameter inside bark, with bark one inch thick, the bark percentages are BTV% = ( ) / 22 2 * 100 = 17.4%. BWV% = ( ) / 20 2 * 100 = 21.0%. This calculation is likely to overestimate the true bark volume because of fissures and voids in the bark. A range of 26 to 28% void volume was found for three softwood species (Krier and River 1968), hence the above results should be reduced by this amount. The recovered bark may be lower, due to miscellaneous losses during harvesting, log handling, and debarking. Smith and Kozak (1967) developed bark thickness regressions for a variety of western Canadian species. Table 75 presents average total bark volume percentages, moisture contents, and specific gravities of inner and outer bark. The bark moisture contents reflect conditions that would normally be found in logs and do not include additional water from pond storage or water added during debarking. 11
12 Hog Fuel Hog fuel is generally a mix of bark, sawdust, and planer shavings. The relative amount of each depends on a particular mill's marketing alternatives for these residues. The mix can be estimated as a weighted average using the information presented in the appropriate yield sections (see Estimating a Hog Fuel Mix below). If an estimate is needed with a high degree of confidence, samples of the hog fuel in question should be analyzed. Residue Calculation Examples Estimating Yield from Plywood The following procedure can be used for lumber, veneer, plywood, and so forth. Assume that it is desired to estimate the number of 200 cubic foot units of chips recovered per 1,000 square feet (3/8 inch basis) of Douglasfir plywood. The average milllength block is 15 inches in diameter. 1. From the plywood material balance studies (Fahey and Willits 1991), about 25% of a milllength veneer block is recovered as chippable residue, and about 50% is recovered as dry veneer. About 12% of the dry veneer will be lost in making plywood, so about 45% of the block will be plywood. 2. Chapter 5 shows that 1,000 square feet, 3/8 inch basis, plywood has a cubic volume of cubic feet. 3. Since the cubic volume of plywood (31.25 ft 3 ) represents 45% of the cubic block volume and since the cubic volume of clean chips represents 25% of the block volume, the solid wood equivalent volume of chips can be estimated by proportions as follows: 45 / = 25 / x. Solving, yields x = 17.4 ft 3 solid equivalent of chips recovered per 1,000 ft 2, 3/8 inch, plywood. 4. Convert the solid chip volume by the compacted chip expansion factor of Table 71. Compacted chips = 17.4 ft 3 solid chips * 2.50 ft 3 compact chips per solid ft 3 = 43.5 ft Since a unit is 200 cubic feet, there are 43.5 / 200 = units of compact chips recovered per 1,000 square feet of 3/8 inch basis plywood. Estimating Yield per Cunit of Log Input Assume a plywood process with the same conditions as indicated above. 1. From the material balance equations (Fahey and Willits 1991), about 25% of a milllength veneer block is recovered as chippable residue. 2. Yield of chips = 100 ft 3 /cunit * 0.25 = 25 ft 3 solid chips. 3. Multiply by the compacted chip expansion factor in Table 71. Compacted chips = 25 ft 3 solid chips * 2.50 ft 3 compact chips per ft 3 solid chips = 62.5 ft Therefore, a cunit of veneer blocks yields 62.5 / 200 = units of compact chips. Converting Units of Residue to Weight How many units of pulp chips equal an ovendry short ton? 1. Assume the species is Douglasfir, which has a SGg of 0.45 (Table 11). Table 12 shows the weight density at 0% MCod, or 28.1 pounds per solid cubic foot. 2. Divide by the compact chip expansion factor (Table 71) to get a bulk density of ovendry lb/ft 3 compact chips. Alternatively, use a bulk density based on samples. 3. Divide 2,000 pounds in a short ton by the bulk density estimate to get the number of cubic feet of compacted chips per short ton: 2,000 / = 178 ft Since a unit is 200 cubic feet, a short ton represents 178 / 200 = 0.89 units under these conditions. Note: Simple division shows that for a 200 cubic foot unit to exactly equal a short ton, the bulk density would be 2,000 / 200 = 10 ovendry lb/ft 3 residue. Similar calculations for other weight measures imply ovendry bulk densities as follows: Long ton BDU Tonne Chapter 7
13 Estimating a Hog Fuel Mix Assume that the hog fuel for a cunit of Douglasfir logs processed in a sawmill will contain all of the sawdust, planer shavings, and bark produced by the mill. 1. From the material balances in Chapter 4 and the bark section in this chapter, assume the following recoveries as percentages of green wood volume: sawdust, 8%; shavings, 5%; bark, 28%. Reduce the bark fraction by 30% to account for fissures, voids, and processing losses so that the net bark fraction is 20%. 2. Column 1 of the table below multiplies these recovery percents by the 100 cubic feet in a cunit to give solid volume yields in cubic feet. 3. Column 2 lists the appropriate residue expansion factors from Table 71, and column 3 is the expanded residue volume in cubic feet after multiplying column 1 by column Columns 4 and 5 present MCod and SGg assumptions. It is assumed that sawdust is generated when processing green wood with an MCod of 80%. The planer shavings are assumed to be generated after kiln drying to an average MCod of 16%. The bark MCod and SGg are weighted averages of inner and outer bark of Douglasfir from Table 75. Columns 6 and 7 are estimates of wet and ovendry solid wood densities using Table Dividing the solid wood densities of columns 6 and 7 by the expansion factors in column 2 results in residue green and dry bulk densities in columns 8 and Multiplying the residue volume in column 3 by the green and dry bulk densities in columns 8 and 9 results in green and dry residue weights in columns 10 and Totals of columns 3, 10, and 11 give the final hog fuel values of interest. For the conditions assumed here, a cunit of logs yields 92 cubic feet (0.46 unit) of hog fuel having a green weight of 1,767 pounds (green bulk density of 19.2 lb/ft 3 ) and ovendry weight of 972 pounds (dry bulk density of 10.6 lb/ft 3 ). The hog fuel is equal to 0.40 BDU. Residue (1) (2) (3) (4) (5) (6) (7) (8) (9) (10) (11) Sawdust Shaving Bark , Total 92 1, Chips 13
14
15 87 Chapter 7
Chapter 3. Stacked Roundwood, PreservativeTreated Products, and Construction Logs
1 Chapter 3. Stacked Roundwood, PreservativeTreated Products, and Construction Logs Stacked Roundwood 38 Cord Measure 38 Standard rough cord Long cord The unit Face cord Volume of solid wood in a cord
More informationWhat Do You See? FOR 274: Forest Measurements and Inventory. Logs and Scaling: Definitions. Tree and Wood Volume Log Volumes Cords Weight Scaling
What Do You See? FOR 274: Forest Measurements and Inventory Tree and Wood Volume Log Volumes Cords Weight Scaling Logs and Scaling: Definitions Logs: cut trees lengths of 8ft or more The process of measuring
More informationChapter 8. Pulp and Paper
Chapter 8. Pulp and Paper Pulp Yield 96 Mechanical Pulping 96 Chemical Pulping 96 Kraft (sulfate) process Sulfite process Hybrid Pulping Methods 97 Dissolving Pulp 97 Estimating Wood Required per Ton of
More informationUnits of Measure and Conversion Factors for Forest Products
Units of Measure and Conversion Factors for Forest Products Bulletin #7103 Knowledge of the common units of wood measurement is important to people who are involved in marketing forest products. These
More informationConversion Factors and Measurement of Biomass Fuels for Nova Scotia
Conversion Factors and Measurement of Biomass Fuels for Nova Scotia Companion to the Discussion Paper: Revisions to Forests Act Regulations Affecting Forest and Wood Biomass Users Revisions to Forests
More informationMeasuring Pulp Logs and Biomass: results of log studies. Matt Fonseca UNECE/FAO Timber Section
Measuring Pulp Logs and Biomass: results of log studies Matt Fonseca UNECE/FAO Timber Section Measuring pulp logs and biomass What does the purchaser want? An accurate predictor of useable fiber What are
More informationChapter 4. Lumber. Lumber 1
Chapter 4. Lumber Nominal and Manufactured Lumber Sizes 52 Softwood Lumber Sizes 52 Construction lumber Lumber for remanufacture Hardwood Lumber Sizes 52 Factory lumber thickness Factory lumber width and
More informationPB Understanding Log Scales and Log Rules
PB 1650 Understanding Log Scales and Log Rules 1 Understanding Log Scales and Log Rules Brian Bond, Former Assistant Professor, Forestry, Wildlife and Fisheries Introduction A necessary step in determining
More informationNew Hampshire Native Lumber Law RSA 434: Self Study Booklet
New Hampshire Native Lumber Law RSA 434:5961 Self Study Booklet Issued by: UNH Cooperative Extension 210 Nesmith Hall, 131 Main St. Durham, NH 03857 Contact: Sarah Smith (603)8622647 sarah.smith@unh.edu
More informationDefinitions of each biomass component and the equations used to estimate the ovendry weight in pounds are shown in appendix tables J1 through J5.
. Biomass Estimation in the FIADB In previous versions of the FIADB, a variety of regional methods were used to estimate tree biomass for live and dead trees in the TREE table. In FIADB 4.0, a new nationally
More informationArbor Day Tree Trivia
Arbor Day Tree Trivia What day is Arbor Day? The last Friday of April. (April 30, 2010) Who is the father of Arbor Day? J. Sterling Morton When was the first Arbor Day? 1872 Name Idaho's state tree. Western
More informationNOTE: FOR PROJECTS REQUIRING CONTRACTOR MIX DESIGN, THE DESIGN PROCEDURES ARE SPECIFIED IN THE SPECIAL PROVISIONS OF THE CONTRACT.
September 1, 2003 CONCRETE MANUAL 5694.300 MIX DESIGN 5694.300 NOTE: FOR PROJECTS REQUIRING CONTRACTOR MIX DESIGN, THE DESIGN PROCEDURES ARE SPECIFIED IN THE SPECIAL PROVISIONS OF THE CONTRACT. 5694.301
More informationFOR 306 Forest measurements. Trees Weight
FOR 306 Forest measurements Trees eight weight Measure of the quantity of wood eight used also for: Scaling Complete tree utilization root, branches or stump Biomass Carbon content Fuel eight determined
More informationThe percentages of clear wood required for each grade are based on this 12' unit of measure.
Introduction The purpose of this publication is to provide a simplified but thorough explanation of the grading rules for American hardwood lumber. They were established over 100 years ago by the newly
More informationSpecific Gravity, Moisture Content, and Density Relationship for Wood
United States Department of Agriculture Forest Service Forest Products Laboratory General Technical Report FPLGTR76 Specific Gravity, Moisture Content, and Density Relationship for Wood William T. Simpson
More informationCHAPTER 4 Moisture Content and its Measurement
CHAPTER 4 Moisture Content and its Measurement Moisture content (MC) is a measure of the amount of water found within a material at any given time. As discussed in Chapter 2, wood has an affinity for moisture
More informationHardwood Lumber Lesson Plan. Keywords: hardwood, softwood, grading, drykiln, sawmill, and board foot
Hardwood Lumber Lesson Plan Keywords: hardwood, softwood, grading, drykiln, sawmill, and board foot Lesson Plan Grade Level: 6 th  8 th Total Time Required For Lesson: 50 minutes (as one continuous time
More informationTHE CASE FOR CUBIC LOG SCALE
Page 1 1. INTRODUCTION THE CASE FOR CUBIC LOG SCALE The history of scaling rules or log scales in the US goes back to the earliest lumbermen of North America. Many proprietary systems were used in the
More informationTree Biomass & Carbon Price & Cost Information. FOR 1001 Dr. Thom Erdle
Tree Biomass & Carbon Price & Cost Information FOR 1001 Dr. Thom Erdle Today s Objectives Meaning and measurement of biomass and carbon Meaning and calculation of stumpage Familiarity with pricing cost
More informationLesson 12: Processing Timber Products
Lesson 12: Processing Timber Products TEACHER: SCHOOL: GRADE LEVEL: 912 TASKS/COMPETENCIES ANR8040.088 Locate markets for forest products. ANR8040.097 Demonstrate ability to operate circular saw. ANR8040.098
More informationEPPO Study on Wood Commodities. Other than round wood, sawn wood and manufactured items
EPPO Study on Wood Commodities Other than round wood, sawn wood and manufactured items Background Identification of different types of commodities + Bark + Isolated bark + Wood + Processed wood material
More informationBulk Density ( Unit Weight ) and Voids in Aggregate
Standard Method of Test for Bulk Density ( Unit Weight ) and Voids in Aggregate AASHTO Designation: T 19M/T 1900 (2004) ASTM Designation: C 29/C 29M97 (2003) 1. SCOPE 1.1. This test method covers the
More informationTimber MartSouth CUT & LOAD CONTRACT RATES. US$ per Ton. Harvest Type LO HI AVG Harvest Type LO HI AVG HAULING RATES
LOGGING RATES PIEDMONT CUT & LOAD CONTRACT RATES US$ per Ton COASTAL PLAIN Harvest Type LO HI AVG Harvest Type LO HI AVG Final Harvest 10.22 14.67 12.44 Final Harvest 9.00 11.45 10.23 Plantation Thin 10.67
More informationHow Can We Measure Trees and Logs for more Useful Information. For: Timber Measurement Society Coeur D Alene, Idaho April 12, 2012
How Can We Measure Trees and Logs for more Useful Information For: Timber Measurement Society Coeur D Alene, Idaho April 12, 2012 By: Toby Atterbury Atterbury Consultants, Inc 3800 SW Cedar Hills Blvd.
More informationCANADIAN MILL SERVICES ASSOCIATION
CANADIAN MILL SERVICES ASSOCIATION CURRICULUM OF EDUCATION PROGRAMS ORGANIZATION HISTORY The formation of Canadian Mill Services Association came about in early 1994 after an indepth review and organization
More informationLUMBER & CHIP SALES (AMV) MONTHLY REPORT INSTRUCTIONS
Monthly reports are to be submitted by the 20th day of the following month. Excel Program CLS Lumber If you are using the Excel program, please note that it is already formatted. All you need to do is
More informationFORECASTING AND MONITORING MOISTURE CONTENT OF WOODY BIOMASS IN IRELAND AND OREGON TO IMPROVE SUPPLY CHAIN ECONOMICS Glen Murphy 1, Francisca Belart 2, Tom Kent 3 and Pieter D. Kofman 4 ABSTRACT Wood is
More informationNHLA GRADING RULES FOR NORTH AMERICAN HARDWOODS
NHLA GRADING RULES FOR NORTH AMERICAN HARDWOODS The NHLA grades are based on the percentage of cleardefect free wood on a board. The measurements of this percentage are referred to as clearcuttings.
More information2012 Indiana Forest Products Price Report and Trend Analysis
PURDUE EXTENSION 2012 Indiana Forest Products Price Report and Trend Analysis William L. Hoover, Professor of Forestry, Department of Forestry and Natural Resources, Purdue University, and Greg Preston,
More informationHow is carbon stored in trees and wood products?
How is carbon stored in trees and wood products? Science S Theory Lesson Lesson information Level: Junior secondary school Year 10 Duration: Summary: Approximately 3 lessons Sustainably managed forests
More informationNATIONAL GRADING RULE FOR SOFTWOOD DIMENSION LUMBER INTERPRETATIONS
NATIONAL GRADING RULE FOR SOFTWOOD DIMENSION LUMBER INTERPRETATIONS Index Part  National Grading Rule for Softwood Dimension Lumber Interpretations.. 59.0 General...5. Bark and Pitch Pockets...5.2 Bevel
More informationSPECIFICATIONS FOR BRIDGE CONSTRUCTION SECTION 23 DIMENSIONAL STRUCTURAL LUMBER AND PILING General Standards...
SPECIFICATIONS FOR BRIDGE CONSTRUCTION SECTION 23 DIMENSIONAL STRUCTURAL LUMBER AND PILING TABLE OF CONTENTS 23.1 General...231 23.2 Standards...231 23.3 Material Specification...231 23.3.1 Planking
More informationLesson 10: Basic Inventory Calculations
Lesson 10: Basic Inventory Calculations Review and Introduction In the preceding lessons, you learned how to establish and take measurements in sample plots. You can use a program like LMS to calculate
More informationFirewood, Facts, Follies and Forest Management
Firewood, Facts, Follies and Forest Management Brian Bond and Adam Downing Virginia Tech College of Natural Resources and Environment Outline Introduction What burns best and why? Species Density Moisture
More informationFACILITY PROFILE J. D. Irving, Limited Chipman Sawmill Chipman, N.B.
FACILITY PROFILE J. D. Irving, Limited Chipman Sawmill Chipman, N.B. Prepared by: Impact Management Branch New Brunswick Department of Environment and Local Government October 2014 TABLE OF CONTENTS BACKGROUND
More informationA Streamlined Approach to the Component Ratio Method for RGGI U.S. Forest Projects Outside of California, Oregon, Washington, Alaska and Hawaii
for RGGI U.S. Forest Projects Outside of California, Oregon, Washington, Alaska and Hawaii May 13, 2015 Background on the Component Ratio Method... 2 Streamlined Approach to the Component Ratio Method...
More informationAlaska Northern Forest Cooperative
Alaska Northern Forest Cooperative Hardwood Management Fall Symposium Overview of Marketing, Testing and Milling of Alaska Birch Lumber Dave Nicholls Wasilla, AK October 12, 2006 USDA Forest Service Pacific
More informationWood Properties Technology
Wood Properties Technology T Practical Lesson Activity information Level: Junior secondary school Years 7 10 Duration: Preparation: Summary: Approximately 2 lessons Collect two samples of timber Students
More informationChapter 4. Mechanical Properties of Wood. Contents. Orthotropic Nature of Wood. David W. Green, Jerrold E. Winandy, and David E.
Mechanical Properties Wood David W. Green, Jerrold E. Winandy, and David E. Kretschmann Chapter 4 Contents Orthotropic Nature Wood 4 1 Elastic Properties 4 2 Elasticity 4 2 Poisson s Ratio 4 2 Rigidity
More informationFOREST PRODUCT CONVERSION FACTORS FOR THE UNECE REGION
UNECE United Nations Economic Commission for Europe Food and Agriculture Organization of the United Nations GENEVA TIMBER AND FOREST DISCUSSION PAPER 49 FOREST PRODUCT CONVERSION FACTORS FOR THE UNECE
More informationSLABS, COLUMNS & FOOTINGS
SLABS, COLUMNS & FOOTINGS Multiply the height of your column by the number that corresponds to the diameter to determine the cubic yards needed. Column CY = 0.78 x A x B 7 B A Diameter CY Diameter CY Diameter
More informationHardwood Lumber Processing
Hardwood Lumber Processing Forest Management Our timber harvesting programs are diverse and can be adapted to a variety of forest management goals. All of our forest management activity is monitored by
More informationForestry Terms. Allowable cut The volume of wood that can be cut during a given period without exceeding the forest s net growth.
Forestry Terms Acre A land area of 43,560 square feet, approximately 209 ft. by 209 ft. Allowable cut The volume of wood that can be cut during a given period without exceeding the forest s net growth.
More informationFlame Spread Performance of Wood Products
Flame Spread Performance of Wood Products Wood and woodbased products are widely used in interior wall, ceiling, and floor surfaces in all types of buildings. Appearance, acoustical qualities, and interior
More informationRECIPIENT OF THE PRESIDENT S E AWARD FOR EXPORTS Visit for details.
RECIPIENT OF THE PRESIDENT S E AWARD FOR EXPORTS Visit www.lumberexport.com for details. www.lumberexport.com A leading worldwide exporter of quality lumber, plywood and poles. A reliable single source
More informationWest Coast Lumber Inspection Bureau
West Coast Lumber Inspection Bureau NGR  08 Interpretations for the National Grading Rules for Dimension Lumber 2008 Approved by: National Grading Rule Committee November 4, 2004 Copyright WCLIB 2008.
More informationAustralian Pine Log Price Index
Australian Pine Log Price Index Updated to June 28 : ADVISORY This page has been intentionally left blank. Advisory This report contains 39 pages HVP8 Jan  Jun (Public Version) 26 KPMG, an Australian
More informationA Log Volume Formula for Exporters
A Log Volume Formula for Exporters J.C. Ellis Summary This paper shows that the volume estimate of export logs would be more accurate using a taper value in the 3D formula than volumes derived from the
More informationChapter 6. Material Estimates
Chapter 6 Material Estimates To obtain a satisfactory surface, combine bituminous materials and aggregate in various proportions. Material estimates must be as accurate as possible to avoid an inadequate
More informationDETERMINING POTENTIAL VERTICAL RISE
Test Procedure for DETERMINING POTENTIAL VERTICAL RISE TxDOT Designation: Tex124E Effective Dates: August 1999 February 2014. 1. SCOPE 1.1 This procedure determines the potential vertical rise (PVR)
More informationValuing Timber Resource Stocks in the Canadian Natural Resource Stock Accounts
Valuing Timber Resource Stocks in the Canadian Natural Resource Stock Accounts London Group, November 2013 Environment Accounts and Statistics Division Statistics Canada October 18 th, 2013 Quick facts
More informationChapter 201 Random Length Lumber Futures
20100. SCOPE OF CHAPTER Chapter 201 Random Length Lumber Futures This chapter is limited in application to Random Length Lumber futures. In addition to this chapter, Random Length Lumber futures shall
More informationWEIGHTS AND MEASURES
WEIGHTS AND MEASURES Tables of Weights and Measures; and other information that may be helpful to the Assessor/Appraiser. Metric Measure Millimeter = 0.001 meter Centimeter = 0.01 meter Decimeter = 0.1
More informationFOREST PRODUCT CONVERSION FACTORS: PROJECT OVERVIEW AND STATUS
10 March 2009 Page 1 FOREST PRODUCT CONVERSION FACTORS: PROJECT OVERVIEW AND STATUS 1. USE OF CONVERSION FACTORS 1.1 Background The term forest products conversion factors is used to cover a broad spectrum
More informationGRADATION OF AGGREGATE FOR CONCRETE BLOCK
GRADATION OF AGGREGATE FOR CONCRETE BLOCK Although numerous papers have been written concerning the proper gradation for concrete mixes, they have generally dealt with plastic mixes, and very little published
More informationUNDERSTANDING REFRIGERANT TABLES
Refrigeration Service Engineers Society 1666 Rand Road Des Plaines, Illinois 60016 UNDERSTANDING REFRIGERANT TABLES INTRODUCTION A Mollier diagram is a graphical representation of the properties of a refrigerant,
More informationThe entire document shall be read and understood before proceeding with a test. ISTA 3B 2013  Page 1 of 35
PackagedProducts for LessThanTruckload (LTL) Shipment ISTA 3 Series General Simulation Performance Test PROCEDURE VERSION DATE Last TECHNICAL Change: NOVEMBER 2012 Last EDITORIAL Change: JANUARY 2013
More informationNTRAL HARDWOOD NOTES. Grading Hardwood Trees
North Central Forest Experiment Station 7.03 NTRAL HARDWOOD NOTES Grading Hardwood Trees Tree grading provides a way to evaluate the quality characteristics and value of standing hardwood trees. This is
More informationFuture Prospects for USA Pulp and Paper Technology. Richard B. Phillips, PhD Student TAPPI Summit Raleigh, North Carolina January 20, 2012
Future Prospects for USA Pulp and Paper Technology Richard B. Phillips, PhD Student TAPPI Summit Raleigh, North Carolina January 20, 2012 Main Points 1. USA very competitive with Rest of the World in Pulp
More informationTimber Harvesting and Longdistance Transportation of Roundwood 2014. Metsätehon tuloskalvosarja 7b/2015 Markus Strandström Metsäteho Oy
Timber Harvesting and Longdistance Transportation of Roundwood 214 Metsätehon tuloskalvosarja 7b/215 Markus Strandström Metsäteho Oy About statistics Includes volumes and direct harvesting costs of timber
More informationTransit Mix Perlite Description Mixing Perlite Concrete Transit Mixing
Transit Mix Perlite Description Perlite concrete aggregate combined with Portland cement, air entraining agent, and water produces an ultra lightweight concrete that is used for insulating roof decks and
More informationUNIT 1 MASS AND LENGTH
UNIT 1 MASS AND LENGTH Typical Units Typical units for measuring length and mass are listed below. Length Typical units for length in the Imperial system and SI are: Imperial SI inches ( ) centimetres
More informationMOISTURE REMOVAL FROM GREEN SAPWOOD DURING PLATEN PRESSING
109 MOISTURE REMOVAL FROM GREEN SAPWOOD DURING PLATEN PRESSING R. WING ATEHILL CSIRO Division of Forest Research, P.O. Box 4008, Canberra, A.C.T. 2600, Australia and R. B. CUNNINGHAM Department of Statistics,
More informationComparison of Logging Residue from Lump Sum and Log Scale Timber Sales James O. Howard and Donald J. DeMars
United States Department of Agriculture Forest Service Pacific Northwest Forest and Range Experiment Station Research Paper PNW337 May 1985 Comparison of Logging Residue from Lump Sum and Log Scale Timber
More informationCONCRETE TECHNOLOGY LABORATORY
CONCRETE TECHNOLOGY LABORATORY DEPARTMENT OF CIVIL ENGINEERING CHULALONGKORN UNIVERSITY Tested by... ID. No.... Date... Graded by... TEST No. C2 PROPERTIES OF AGGREGATE Part A Specific Gravity and Absorption
More information2009 JULY TIMBER SALES
2009 JULY TIMBER SALES FLAMBEAU RIVER STATE FOREST W1613 COUNTY ROAD W WINTER, WI 54896 (715) 3325271 Sealed bids will be received by the Wisconsin Department of Natural Resources, Flambeau River State
More informationSMALLSCALE LUMBER DRYING USING WOOD GASIFICATION AS A HEAT SOURCE
SMALLSCALE LUMBER DRYING USING WOOD GASIFICATION AS A HEAT SOURCE Richard D. Bergman USDA Forest Service Madison, Wisconsin ABSTRACT Small, rural forested communities have the economic need to develop
More informationCONVERSIONS AND STATISTICS
CONVERSIONS AND STATISTICS Approximate Conversion Factors for Estimating Purposes (Compacted) Granular A, M 2.2 tonnes/m 3, 2.0 tons/yd 3 Granular B 2.1 tonnes/m 3, 1.8 tons/yd 3 3/4 Crushed Gravel (Clear)
More informationhp calculators HP 35s Unit Conversions Metric units and Imperial units Conversion keys Practice working problems involving conversions
Metric units and Imperial units Conversion keys Practice working problems involving conversions Performing conversions that are not built in Special considerations for temperature conversions Metric units
More informationFACTORS WHICH INFLUENCE COMPANIES IN FOREST MANAGEMENT DECISIONS
292 Vol. 6 FACTORS WHICH INFLUENCE COMPANIES IN FOREST MANAGEMENT DECISIONS B. D. McCONCHIE J. G. Groome and Associates, Taupo, New Zealand ABSTRACT Factors which generally influence companies in making
More informationForest Resources of the Gila National Forest
United States Department of Agriculture Forest Service Rocky Mountain Research Station May 2008 Forest Resources of the Gila National Forest John D. Shaw New Mexico Gila National Forest About the author
More informationSTATE OF OHIO DEPARTMENT OF TRANSPORTATION SUPPLEMENT 1015 COMPACTION TESTING OF UNBOUND MATERIALS. July 18, 2014
STATE OF OHIO DEPARTMENT OF TRANSPORTATION SUPPLEMENT 1015 COMPACTION TESTING OF UNBOUND MATERIALS July 18, 2014 1015.01 General 1015.02 Definitions 1015.03 Referenced Standards 1015.04 Equipment 1015.05
More informationRenewable Energy from Biomass. Opportunities in London and Area? Eric Rosen
Renewable Energy from Biomass Opportunities in London and Area? Eric Rosen KMW ENERGY INC. LONDON, ONTARIO Tel: (519) 6861771 www.kmwenergy.com Company Background Long History in designing bioenergy systems.
More informationGATETOGATE LIFECYCLE INVENTORY OF SOFTWOOD LUMBER PRODUCTION. Michael R. Milota. Cynthia D. West. Ian D. Hartley
GATETOGATE LIFECYCLE INVENTORY OF SOFTWOOD LUMBER PRODUCTION Michael R. Milota Professor Department of Wood Science and Engineering Oregon State University Corvallis, OR 97331 Cynthia D. West Assistant
More informationDesigning with Lumber in the 2001 NDS
Designing with Lumber in the 2001 NDS Kevin Cheung, Scott Lockyear, Eric Jones, Don DeVisser, and Lisa Johnson Abstract The National Design Specification (NDS ) for Wood Construction, 2001 Edition, an
More information$2.50 PB1772. A Hardwood Log Grading Handbook
$2.50 PB1772 A Hardwood Log Grading Handbook Contents How Much Is a Log Worth?...1 Veneer, Sawlogs and Other Log Classes...2 Log Scaling...3 Table 1. The Doyle Log Rule...4 Log Grading Relation to Lumber
More informationOPTIMIZED PERFORMANCE FOR WOOD PROCESSING.
OPTIMIZED PERFORMANCE FOR WOOD PROCESSING. GLOBALLY PROVEN EXPERTISE IN OPTIMIZATION Teknosavo is specialized in delivering optimization systems and online measurement systems for wood processing industries
More informationDIRECT FIRED DRYING VERSUS STEAM DRYING OF LUMBER
DIRECT FIRED DRYING VERSUS STEAM DRYING OF LUMBER Mr. Robert Beckly, Products Manager Moore Dry Kiln Company of Oregon North Portland, Oregon There has been some confusion in the past regarding the subject
More informationEnergy Profiling in Sawmills
Dayakar Devaru, Ph.D Student Ramakrishna Babu Maddula, Ph.D Student Dr. Bhaskaran Gopalakrishnan Director of Industrial Assessment Center Sawmills are a major sector of the wood industry that transform
More informationMultiplying Decimal Numbers by 10, by 100, and by 1000
Multiplying Decimal Numbers by 10, by 100, and by 1000 Lesson 111 111 To multiply by 10, shift the decimal to the right one place. To multiply by 100, shift the decimal to the right two places. To multiply
More information
Unit Conversions. Ben Logan Feb 10, 2005
Unit Conversions Ben Logan Feb 0, 2005 Abstract Conversion between different units of measurement is one of the first concepts covered at the start of a course in chemistry or physics.
More informationPRESERVATIVE TREATMENT 06076
PO Drawer O 1016 Everee Inn Road Griffin, GA 302240249 Phone: (800) 2410240 Phone: (770) 2334200 Fax: (770) 2295225 Email: treatedwood@osmose.com www.osmose.com This MANUSPEC utilizes the Construction
More informationWood fuels: pellets and chips
Wood fuels: pellets and chips Robinwood International Wood Energy Week Eberswalde Polytechnic, 23th January 2006 Anssi Kokkonen North Karelia Polytechnic Joensuu, Finland North Karelia North Karelia Polytechnic
More informationRed Alder Kitchen Cabinets How Does Application of Commercial Stains Influence Customer Choice?
United States Department of Agriculture Forest Service Pacific Northwest Research Station Research Note PNWRN556 Red Alder Kitchen Cabinets How Does Application of Commercial Stains Influence Customer
More informationMeasure particle density, bulk density, and moisture content of a soil and to relate to total pore space.
LABORATORY 2 SOIL DENSITY I Objectives Measure particle density, bulk density, and moisture content of a soil and to relate to total pore space. II Introduction A Soil particle density (g / cm 3 ) is mass
More informationINTERGOVERNMENTAL STANDARD GOST 3916.196
INTERGOVERNMENTAL STANDARD GOST 3916.196 Plywood with outer layers of deciduous veneer for general use. Contents DESCRIPTION GENERAL USE PWOOD CLASSIFICATION AND DIMENSIONS( table1,2) TECHICAL REQUIREMENTS
More informationGrammage of paper and paperboard (weight per unit area) (Revision of T 410 om08) (underscores and strikeouts indicate changes from Draft 1)
NOTICE: This is a DRAFT of a TAPPI Standard in ballot. Although available for public viewing, it is still under TAPPI s copyright and may not be reproduced or distributed without permission of TAPPI. This
More informationTimber Products Inspection, Inc.
Timber Products Inspection, Inc. Log Program Technical Guide (02/01/08) Technical Guide Table of Contents Page i Table of Contents Introduction 1 TP Log Program Overview 2 Definition of Stress Grades Description
More informationValue chain modeling and pulp and paper industry competitiveness
Value chain modeling and pulp and paper industry competitiveness UBC March 23, 2007 Research Seminar facilitated by the BC Forum on Forest Economics and Policy Outline Paprican and FPInnovations Fibre
More informationWoodMizer Sawmill. General Information. Basic concepts regarding sawing and drying lumber. March 2002 Form #601
WoodMizer Sawmill General Information Basic concepts regarding sawing and drying lumber Safety is our #1 concern! Read and understand all safety information and instructions before operating, setting
More informationLandEnergy Girvan Low carbon wood pellet production 28 September 2012
LandEnergy Girvan Low carbon wood pellet production 28 September 2012 Biography Hugh Montgomery Joined Land Energy as Business Development Manager in 2008. During three years in the oil and gas sector,
More informationTHE CORPORATION OF THE TOWN OF MIDLAND DECK PERMIT GUIDELINES
THE CORPORATION OF THE TOWN OF MIDLAND DECK PERMIT GUIDELINES BUILDING DEPARTMENT Planning and Building Services 575 Dominion Avenue Midland, ON L4R 1R2 Tel: 705 526 4275 Fax: 705 526 9971 www.midland.ca
More informationTHE NATURE OF THE WOOD PELLET SUPPLY TO THE UK
THE NATURE OF THE WOOD PELLET SUPPLY TO THE UK Carly Whittaker Rothamsted Research Torrefaction workshop 2 nd April 2014 University of Leeds Rothamsted Research MSc Forest Protection and conservation at
More informationRegional Analysis of Woody Biomass Resources. North Carolina s Southeast Region
Regional Analysis of Woody Biomass Resources North Carolina s Southeast Region Prepared by: Gelbert, Fullbright & Randolph Forestry Consultants, PLLC 8394 Six Forks Road, Suite 23 Raleigh, North Carolina
More informationHome Heating Fuels. Should I switch to firewood or wood pellets?
EC 1628E June 2009 Home Heating Fuels Should I switch to firewood or wood pellets? J. Reeb With rising costs for natural gas, fuel oil, and electricity, more people are thinking of burning firewood or
More informationCHAPTER 2 HYDRAULICS OF SEWERS
CHAPTER 2 HYDRAULICS OF SEWERS SANITARY SEWERS The hydraulic design procedure for sewers requires: 1. Determination of Sewer System Type 2. Determination of Design Flow 3. Selection of Pipe Size 4. Determination
More informationBiomass availability and supply for cofiring projects in Alberta. Dominik Roser, Ph.D.
Biomass availability and supply for cofiring projects in Alberta Dominik Roser, Ph.D. About FPInnovations A private nonprofit Canadian corporation Supports competitiveness of the Canadian forest sector
More informationFractions, Ratios, and Proportions Work Sheets. Contents
Fractions, Ratios, and Proportions Work Sheets The work sheets are grouped according to math skill. Each skill is then arranged in a sequence of work sheets that build from simple to complex. Choose the
More informationAmerican Forest & Paper Association American Wood Council
2005 EDITION S U P P L E M E N T N D S n a t i o n a l d e s i g n s p e c i f i c a t i o n DESIGN VALUES FOR WOOD CONSTRUCTION American Forest & Paper Association American Wood Council Updates and Errata
More information